Semiconductors CHAPTER 3. Introduction The pn Junction with an Applied Voltage Intrinsic Semiconductors 136


 Frederick Randall
 4 years ago
 Views:
Transcription
1 CHAPTER 3 Semiconductors Introduction Intrinsic Semiconductors Doped Semiconductors Current Flow in Semiconductors The pn Junction The pn Junction with an Applied Voltage Capacitive Effects in the pn Junction 164 Summary 168 Problems 171
2 IN THIS CHAPTER YOU WILL LEARN 1. The basic properties of semiconductors and in particular silicon, which is the material used to make most of today s electronic circuits. 2. How doping a pure silicon crystal dramatically changes its electrical conductivity, which is the fundamental idea underlying the use of semiconductors in the implementation of electronic devices. 3. The two mechanisms by which current flows in semiconductors: drift and diffusion of charge carriers. 4. The structure and operation of the pn junction; a basic semiconductor structure that implements the diode and plays a dominant role in transistors. Introduction Thus far we have dealt with electronic circuits, and notably amplifiers, as system building blocks. For instance, in Chapter 2 we learned how to use op amps to design interesting and useful circuits, taking advantage of the terminal characteristics of the op amp and without any knowledge of what is inside the opamp package. Though interesting and motivating, this approach has its limitations. Indeed, to achieve our goal of preparing the reader to become a proficient circuit designer, we have to go beyond this blackbox or systemlevel abstraction and learn about the basic devices from which electronic circuits are assembled, namely, diodes (Chapter 4) and transistors (Chapters 5 and 6). These solidstate devices are made using semiconductor materials, predominantly silicon. In this chapter, we briefly introduce the properties and physics of semiconductors. The objective is to provide a basis for understanding the physical operation of diodes and transistors in order to enable their effective use in the design of circuits. Although many of the concepts studied in this chapter apply to semiconductor materials in general, our treatment is heavily biased toward silicon, simply because it is the material used in the vast majority of microelectronic circuits. To complement the material presented here, Appendix A provides a description of the integratedcircuit fabrication process. As discussed in Appendix A, whether our circuit consists of a single transistor or is an integrated circuit containing more than 2 billion transistors, it is fabricated in a single silicon crystal, which gives rise to the name monolithic circuit. This chapter therefore begins with a study of the crystal structure of semiconductors and introduces the two types of charge carriers available for current conduction: electrons and holes. The most significant property of semiconductors is that their conductivity can be varied over a very wide range through the introduction of 135
3 136 Chapter 3 Semiconductors controlled amounts of impurity atoms into the semiconductor crystal in a process called doping. Doped semiconductors are discussed in Section 3.2. This is followed by the study in Section 3.3 of the two mechanisms for current flow in semiconductors, namely, carrier drift and carrier diffusion. Armed with these basic semiconductor concepts, we spend the remainder of the chapter on the study of an important semiconductor structure: the pn junction. In addition to being essentially a diode, the pn junction is the basic element of the bipolar junction transistor (BJT, Chapter 6) and plays an important role in the operation of fieldeffect transistors (FETs, Chapter 5). 3.1 Intrinsic Semiconductors As their name implies, semiconductors are materials whose conductivity lies between that of conductors, such as copper, and insulators, such as glass. There are two kinds of semiconductors: singleelement semiconductors, such as germanium and silicon, which are in group IV in the periodic table; and compound semiconductors, such as galliumarsenide, which are formed by combining elements from groups III and V or groups II and VI. Compound semiconductors are useful in special electronic circuit applications as well as in applications that involve light, such as lightemitting diodes (LEDs). Of the two elemental semiconductors, germanium was used in the fabrication of very early transistors (late 1940s, early 1950s). It was quickly supplanted, however, with silicon, on which today s integratedcircuit technology is almost entirely based. For this reason, we will deal mostly with silicon devices throughout this book. 1 A silicon atom has four valence electrons, and thus it requires another four to complete its outermost shell. This is achieved by sharing one of its valence electrons with each of its four neighboring atoms. Each pair of shared electrons forms a covalent bond. The result is that a crystal of pure or intrinsic silicon has a regular lattice structure, where the atoms are held in their position by the covalent bonds. Figure 3.1 shows a twodimensional representation of such a structure. At sufficiently low temperatures, approaching absolute zero (0 K), all the covalent bonds are intact and no electrons are available to conduct electric current. Thus, at such low temperatures, the intrinsic silicon crystal behaves as an insulator. At room temperature, sufficient thermal energy exists to break some of the covalent bonds, a process known as thermal generation. As shown in Fig. 3.2, when a covalent bond is broken, an electron is freed. The free electron can wander away from its parent atom, and it becomes available to conduct electric current if an electric field is applied to the crystal. As the electron leaves its parent atom, it leaves behind a net positive charge, equal to the magnitude of the electron charge. Thus, an electron from a neighboring atom may be attracted to this positive charge, and leaves its parent atom. This action fills up the hole that existed in the ionized atom but creates a new hole in the other atom. This process may repeat itself, with the result that we effectively have a positively charged carrier, or hole, moving through the silicon crystal structure and being available to conduct electric current. The charge of a hole is equal in magnitude to the charge of an electron. We can thus see that as temperature increases, more covalent bonds are broken and electron hole pairs are generated. The increase in the numbers of free electrons and holes results in an increase in the conductivity of silicon. 1 An exception is the subject of gallium arsenide (GaAs) circuits, which though not covered in this edition of the book, is studied in some detail in material provided on the text website.
4 3.1 Intrinsic Semiconductors 137 Valence electrons Covalent bonds Silicon atoms Figure 3.1 Twodimensional representation of the silicon crystal. The circles represent the inner core of silicon atoms, with +4 indicating its positive charge of +4q, which is neutralized by the charge of the four valence electrons. Observe how the covalent bonds are formed by sharing of the valence electrons. At 0 K, all bonds are intact and no free electrons are available for current conduction. Valence electrons Free electron Broken covalent bond 0 Hole Covalent bond Silicon atoms Figure 3.2 At room temperature, some of the covalent bonds are broken by thermal generation. Each broken bond gives rise to a free electron and a hole, both of which become available for current conduction. Thermal generation results in free electrons and holes in equal numbers and hence equal concentrations, where concentration refers to the number of charge carriers per unit volume (cm 3 ). The free electrons and holes move randomly through the silicon crystal structure, and in the process some electrons may fill some of the holes. This process, called recombination, results in the disappearance of free electrons and holes. The recombination rate is
5 138 Chapter 3 Semiconductors proportional to the number of free electrons and holes, which in turn is determined by the thermal generation rate. The latter is a strong function of temperature. In thermal equilibrium, the recombination rate is equal to the generation rate, and one can conclude that the concentration of free electrons n is equal to the concentration of holes p, n = p = n i (3.1) where n i denotes the number of free electrons and holes in a unit volume (cm 3 ) of intrinsic silicon at a given temperature. Results from semiconductor physics gives n i as n i = BT 3/2 e E g /2kT (3.2) where B is a materialdependent parameter that is cm 3 K 3/2 for silicon; T is the temperature in K; E g, a parameter known as the bandgap energy, is 1.12 electron volt (ev) for silicon 2 ; and k is Boltzmann s constant ( ev/k). It is interesting to know that the bandgap energy E g is the minimum energy required to break a covalent bond and thus generate an electronhole pair. Example 3.1 Calculate the value of n i for silicon at room temperature (T 300 K). Solution Substituting the values given above in Eq. (3.2) provides n i = (300) 3/2 e 1.12/ ( ) = carriers/cm 3 Although this number seems large, to place it into context note that silicon has atoms/cm 3. Thus at room temperature only one in about atoms is ionized and contributing a free electron and a hole! Finally, it is useful for future purposes to express the product of the hole and freeelectron concentration as pn = n 2 i (3.3) where for silicon at room temperature, n i /cm 3. As will be seen shortly, this relationship extends to extrinsic or doped silicon as well. 2 Note that 1 ev = J.
6 3.2 Doped Semiconductors 139 LCDs, THE FACE OF ELECTRONICS: The existence of liquid crystals whose color could be changed by means of an external heat source was first reported in 1888 by an Austrian botanical physiologist. The LC idea lay dormant until the late 1940s, however. Subsequent developments in the field of solidstate electronics provided the technology to harness the technique in display media, with the first LCDs being demonstrated by RCA beginning in Today, LCDs are an essential component in every mobile device as the interface to the world of electronics within. At the other end of the scale, large LCDs are used in flatpanel TVs, and very large LCDs are appearing as dynamic wallpaper in museum display settings. EXERCISE 3.1 Calculate the intrinsic carrier density n i for silicon at T = 50 K and 350 K. Ans /cm 3 ; /cm Doped Semiconductors The intrinsic silicon crystal described above has equal concentrations of free electrons and holes, generated by thermal generation. These concentrations are far too small for silicon to conduct appreciable current at room temperature. Also, the carrier concentrations and hence the conductivity are strong functions of temperature, not a desirable property in an electronic device. Fortunately, a method was developed to change the carrier concentration in a semiconductor crystal substantially and in a precisely controlled manner. This process is known as doping, and the resulting silicon is referred to as doped silicon. Doping involves introducing impurity atoms into the silicon crystal in sufficient numbers to substantially increase the concentration of either free electrons or holes but with little or no change in the crystal properties of silicon. To increase the concentration of free electrons, n, silicon is doped with an element with a valence of 5, such as phosphorus. The resulting doped silicon is then said to be of n type. To increase the concentration of holes, p, silicon is doped with an element having a valence of 3, such as boron, and the resulting doped silicon is said to be of p type. Figure 3.3 shows a silicon crystal doped with phosphorus impurity. The dopant (phosphorus) atoms replace some of the silicon atoms in the crystal structure. Since the phosphorus atom has five electrons in its outer shell, four of these electrons form covalent bonds with the neighboring atoms, and the fifth electron becomes a free electron. Thus each phosphorus atom donates a free electron to the silicon crystal, and the phosphorus impurity is called a donor. It should be clear, though, that no holes are generated by this process. The net positive charge associated with the phosphorus atom is a bound charge that does not move through the crystal. If the concentration of donor atoms is N D, where N D is usually much greater than n i, the concentration of free electrons in the ntype silicon will be n n N D (3.4)
7 140 Chapter 3 Semiconductors Valence electrons Covalent bonds Free electron donated by impurity atom Pentavalent impurity atom (donor) Silicon atoms Figure 3.3 A silicon crystal doped by a pentavalent element. Each dopant atom donates a free electron and is thus called a donor. The doped semiconductor becomes n type. where the subscript n denotes ntype silicon. Thus n n is determined by the doping concentration and not by temperature. This is not the case, however, for the hole concentration. All the holes in the ntype silicon are those generated by thermal ionization. Their concentration p n can be found by noting that the relationship in Eq. (3.3) applies equally well for doped silicon, provided thermal equilibrium is achieved. Thus for ntype silicon p n n n = n 2 i Substituting for n n from Eq. (3.4), we obtain for p n p n n2 i N D (3.5) Thus p n will have the same dependence on temperature as that of n 2 i. Finally, we note that in ntype silicon the concentration of free electrons n n will be much larger than that of holes. Hence electrons are said to be the majority charge carriers and holes the minority charge carriers in ntype silicon. To obtain ptype silicon in which holes are the majority charge carriers, a trivalent impurity such as boron is used. Figure 3.4 shows a silicon crystal doped with boron. Note that the boron atoms replace some of the silicon atoms in the silicon crystal structure. Since each boron atom has three electrons in its outer shell, it accepts an electron from a neighboring atom, thus forming covalent bonds. The result is a hole in the neighboring atom and a bound negative charge at the acceptor (boron) atom. It follows that each acceptor atom provides a hole. If the acceptor doping concentration is N A, where N A n i, the hole concentration becomes p p N A (3.6) where the subscript p denotes ptype silicon. Thus, here the majority carriers are holes and their concentration is determined by N A. The concentration of minority electrons can be found
8 3.2 Doped Semiconductors 141 Valence electrons Covalent bonds Silicon atom Trivalent impurity atom (acceptor) Electron accepted from this atom, thus creating a hole Figure 3.4 A silicon crystal doped with boron, a trivalent impurity. Each dopant atom gives rise to a hole, and the semiconductor becomes p type. by using the relationship and substituting for p p from Eq. (3.6), p p n p = n 2 i n p n2 i N A (3.7) Thus, the concentration of the minority electrons will have the same temperature dependence as that of n 2 i. It should be emphasized that a piece of ntype or ptype silicon is electrically neutral; the charge of the majority free carriers (electrons in the ntype and holes in the ptype silicon) are neutralized by the bound charges associated with the impurity atoms. Example 3.2 Consider an ntype silicon for which the dopant concentration N D = /cm 3. Find the electron and hole concentrations at T = 300 K. Solution The concentration of the majority electrons is n n N D = /cm 3
9 142 Chapter 3 Semiconductors Example 3.2 continued The concentration of the minority holes is p n n2 i N D In Example 3.1 we found that at T = 300 K, n i = /cm 3. Thus, ( ) 2 p n = = /cm 3 Observe that n n n i and that n n is vastly higher than p n. EXERCISES 3.2 For the situation in Example 3.2, find the electron and hole concentrations at 350 K. You may use the value of n i at T = 350 K found in Exercise 3.1. Ans. n n = /cm 3, p n = /cm For a silicon crystal doped with boron, what must N A be if at T = 300 K the electron concentration drops below the intrinsic level by a factor of 10 6? Ans. N A = /cm Current Flow in Semiconductors There are two distinctly different mechanisms for the movement of charge carriers and hence for current flow in semiconductors: drift and diffusion Drift Current When an electrical field E is established in a semiconductor crystal, holes are accelerated in the direction of E, and free electrons are accelerated in the direction opposite to that of E. This situation is illustrated in Fig The holes acquire a velocity ν pdrift given by ν pdrift = μ p E (3.8) where μ p is a constant called the hole mobility: It represents the degree of ease by which holes move through the silicon crystal in response to the electrical field E. Since velocity has the units of centimeters per second and E has the units of volts per centimeter, we see from Eq. (3.8) that the mobility μ p must have the units of centimeters squared per voltsecond (cm 2 /V s). For intrinsic silicon μ p = 480 cm 2 /V s.
10 3.3 Current Flow in Semiconductors 143 E V Holes Electrons x Figure 3.5 An electric field E established in a bar of silicon causes the holes to drift in the direction of E and the free electrons to drift in the opposite direction. Both the hole and electron drift currents are in the direction of E. The free electrons acquire a drift velocity ν ndrift given by ν ndrift = μ n E (3.9) where the result is negative because the electrons move in the direction opposite to E. Here μ n is the electron mobility, which for intrinsic silicon is about 1350 cm 2 /V s. Note that μ n is about 2.5 times μ p, signifying that electrons move with much greater ease through the silicon crystal than do holes. Let s now return to the singlecrystal silicon bar shown in Fig Let the concentration of holes be p and that of free electrons n. We wish to calculate the current component due to the flow of holes. Consider a plane perpendicular to the x direction. In one second, the hole charge that crosses that plane will be (Aqpν pdrift ) coulombs, where A is the crosssectional area of the silicon bar and q is the magnitude of electron charge. This then must be the hole component of the drift current flowing through the bar, I p = Aqpν pdrift (3.10) Substituting for ν pdrift from Eq. (3.8), we obtain I p = Aqpμ p E We are usually interested in the current density J p, which is the current per unit crosssectional area, J p = I p A = qpμ pe (3.11) The current component due to the drift of free electrons can be found in a similar manner. Note, however, that electrons drifting from right to left result in a current component from left to right. This is because of the convention of taking the direction of current flow as the direction of flow of positive charge and opposite to the direction of flow of negative charge. Thus, I n = Aqnν ndrift Substituting for ν ndrift from Eq. (3.9), we obtain the current density J n = I n /A as J n = qnμ n E (3.12) The total drift current density can now be found by summing J p and J n from Eqs. (3.11) and (3.12), J = J p + J n = q ( ) pμ p + nμ n E (3.13) This relationship can be written as J = σ E (3.14)
11 144 Chapter 3 Semiconductors or where the conductivity σ is given by and the resistivity ρ is given by J = E/ρ (3.15) σ = q ( pμ p + nμ n ) (3.16) ρ 1 σ = 1 q ( pμ p + nμ n ) (3.17) Observe that Eq. (3.15) is a form of Ohm s law and can be written alternately as ρ = E J (3.18) Thus the units of ρ are obtained from: V/cm A/cm 2 = cm. Example 3.3 Find the resistivity of (a) intrinsic silicon and (b) ptype silicon with N A = /cm 3. Use n i = /cm 3, and assume that for intrinsic silicon μ n = 1350 cm 2 /V s and μ p = 480 cm 2 /V s, and for the doped silicon μ n = 1110 cm 2 /V s and μ p = 400 cm 2 /V s. (Note that doping results in reduced carrier mobilities.) Solution (a) For intrinsic silicon, p = n = n i = /cm 3 Thus, ρ = ρ = 1 q ( pμ p + nμ n ) ( ) = cm (b) For the ptype silicon p p N A = /cm 3 n p n2 i N A = ( ) = /cm 3
12 3.3 Current Flow in Semiconductors 145 Thus, ρ = = 1 q ( pμ p + nμ n ) ( ) 1 = 1.56 cm Observe that the resistivity of the ptype silicon is determined almost entirely by the doping concentration. Also observe that doping the silicon reduces its resistivity by a factor of about 10 4, a truly remarkable change. EXERCISE 3.4 A uniform bar of ntype silicon of 2μm length has a voltage of 1 V applied across it. If N D = /cm 3 and μ n = 1350 cm 2 /V s, find (a) the electron drift velocity, (b) the time it takes an electron to cross the 2μm length, (c) the driftcurrent density, and (d) the drift current in the case that the silicon bar has a crosssectional area of 0.25 μm 2. Ans cm/s; 30 ps; A/cm 2 ;27μA Diffusion Current Carrier diffusion occurs when the density of charge carriers in a piece of semiconductor is not uniform. For instance, if by some mechanism the concentration of, say, holes, is made higher in one part of a piece of silicon than in another, then holes will diffuse from the region of high concentration to the region of low concentration. Such a diffusion process is like that observed if one drops a few ink drops in a waterfilled tank. The diffusion of charge carriers gives rise to a net flow of charge, or diffusion current. As an example, consider the bar of silicon shown in Fig. 3.6(a): By some unspecified process, we have arranged to inject holes into its left side. This continuous hole injection gives rise to and maintains a hole concentration profile such as that shown in Fig. 3.6(b). This profile in turn causes holes to diffuse from left to right along the silicon bar, resulting in a hole current in the x direction. The magnitude of the current at any point is proportional to the slope of the concentration profile, or the concentration gradient, at that point, J p = qd p dp(x) dx (3.19)
13 146 Chapter 3 Semiconductors Hole injection (a) x Hole concentration, p Hole diffusion Hole current 0 (b) x Figure 3.6 A bar of silicon (a) into which holes are injected, thus creating the hole concentration profile along the x axis, shown in (b). The holes diffuse in the positive direction of x and give rise to a hole diffusion current in the same direction. Note that we are not showing the circuit to which the silicon bar is connected. Electron concentration, n 0 Electron diffusion Electron current x Figure 3.7 If the electron concentration profile shown is established in a bar of silicon, electrons diffuse in the x direction, giving rise to an electron diffusion current in the negativex direction. where J p is the holecurrent density (A/cm 2 ), q is the magnitude of electron charge, D p is a constant called the diffusion constant or diffusivity of holes; and p(x) is the hole concentration at point x. Note that the gradient (dp/dx) is negative, resulting in a positive current in the x direction, as should be expected. In the case of electron diffusion resulting from an electron concentration gradient (see Fig. 3.7), a similar relationship applies, giving the electroncurrent density, dn(x) J n = qd n (3.20) dx where D n is the diffusion constant or diffusivity of electrons. Observe that a negative (dn/dx) gives rise to a negative current, a result of the convention that the positive direction of current is taken to be that of the flow of positive charge (and opposite to that of the flow of negative
14 3.3 Current Flow in Semiconductors 147 charge). For holes and electrons diffusing in intrinsic silicon, typical values for the diffusion constants are D p = 12 cm 2 /s and D n = 35 cm 2 /s. At this point the reader is probably wondering where the diffusion current in the silicon bar in Fig. 3.6(a) goes. A good question, as we are not showing how the rightside end of the bar is connected to the rest of the circuit. We will address this and related questions in detail in our discussion of the pn junction in later sections. Example 3.4 Consider a bar of silicon in which a hole concentration profile described by p(x) = p 0 e x/l p is established. Find the holecurrent density at x = 0. Let p 0 = /cm 3, L p = 1 μm, and D p = 12 cm 2 /s. If the crosssectional area of the bar is 100 μm 2, find the current I p. Solution dp(x) J p = qd p dx d [ ] = qd p p dx 0 e x/l p = q D p L p p 0 e x/l p Thus, The current I p can be found from J p (0) = q D p L p p 0 = = 192 A/cm 2 I p = J p A = = 192 μa EXERCISE 3.5 The linear electronconcentration profile shown in Fig. E3.5 has been established in a piece of silicon. If n 0 = /cm 3 and W = 1 μm, find the electroncurrent density in microamperes per micron squared (μa/μm 2 ). If a diffusion current of 1 ma is required, what must the crosssectional area (in a direction perpendicular to the page) be? Recall that D n = 35 cm 2 /s.
15 148 Chapter 3 Semiconductors n(x) n 0 0 W x Figure E3.5 Ans. 56 μa/μm 2 ;18μm Relationship between D and μ A simple but powerful relationship ties the diffusion constant with the mobility, D n μ n = D p μ p = V T (3.21) where V T = kt/q. The parameter V T is known as the thermal voltage. At room temperature, T 300 K and V T = 25.9 mv. We will encounter V T repeatedly throughout this book. The relationship in Eq. (3.21) is known as the Einstein relationship. EXERCISE 3.6 Use the Einstein relationship to find D n and D p for intrinsic silicon using μ n = 1350 cm 2 /V s and μ p = 480 cm 2 /V s. Ans. 35 cm 2 /s; 12.4 cm 2 /s 3.4 The pn Junction Having learned important semiconductor concepts, we are now ready to consider our first practical semiconductor structure the pn junction. As mentioned previously, the pn junction implements the diode (Chapter 4) and plays the dominant role in the structure and operation of the bipolar junction transistor (BJT, Chapter 6). As well, understanding pn junctions is very important to the study of the MOSFET operation (Chapter 5).
16 3.4 The pn Junction 149 Metal contact Metal contact Anode ptype silicon ntype silicon Cathode Figure 3.8 Simplified physical structure of the pn junction. (Actual geometries are given in Appendix A.) As the pn junction implements the junction diode, its terminals are labeled anode and cathode Physical Structure Figure 3.8 shows a simplified physical structure of the pn junction. It consists of a ptype semiconductor (e.g., silicon) brought into close contact with an ntype semiconductor material (also silicon). In actual practice, both the p and n regions are part of the same silicon crystal; that is, the pn junction is formed within a single silicon crystal by creating regions of different dopings (p and n regions). Appendix A provides a description of the fabrication process of integrated circuits including pn junctions. As indicated in Fig. 3.8, external wire connections are made to the p and n regions through metal (aluminum) contacts. If the pn junction is used as a diode, these constitute the diode terminals and are therefore labeled anode and cathode in keeping with diode terminology Operation with OpenCircuit Terminals Figure 3.9 shows a pn junction under opencircuit conditions that is, the external terminals are left open. The + signs in the ptype material denote the majority holes. The charge of these holes is neutralized by an equal amount of bound negative charge associated with the acceptor atoms. For simplicity, these bound charges are not shown in the diagram. Also not shown are the minority electrons generated in the ptype material by thermal ionization. In the ntype material the majority electrons are indicated by signs. Here also, the bound positive charge, which neutralizes the charge of the majority electrons, is not shown in order to keep the diagram simple. The ntype material also contains minority holes generated by thermal ionization but not shown in the diagram. The Diffusion Current I D Because the concentration of holes is high in the p region and low in the n region, holes diffuse across the junction from the p side to the n side. Similarly, electrons diffuse across the junction from the n side to the p side. These two current components add together to form the diffusion current I D, whose direction is from the p side to the n side, as indicated in Fig The Depletion Region The holes that diffuse across the junction into the n region quickly recombine with some of the majority electrons present there and thus disappear from the scene. This recombination process results also in the disappearance of some free electrons from the 3 This terminology in fact is a carryover from that used with vacuumtube technology, which was the technology for making diodes and other electronic devices until the invention of the transistor in This event ushered in the era of solidstate electronics, which changed not only electronics, communications, and computers but indeed the world!
17 150 Chapter 3 Semiconductors E (b) Figure 3.9 (a) The pn junction with no applied voltage (opencircuited terminals). (b) The potential distribution along an axis perpendicular to the junction. ntype material. Thus some of the bound positive charge will no longer be neutralized by free electrons, and this charge is said to have been uncovered. Since recombination takes place close to the junction, there will be a region close to the junction that is depleted of free electrons and contains uncovered bound positive charge, as indicated in Fig The electrons that diffuse across the junction into the p region quickly recombine with some of the majority holes there, and thus disappear from the scene. This results also in the disappearance of some majority holes, causing some of the bound negative charge to be uncovered (i.e., no longer neutralized by holes). Thus, in the p material close to the junction, there will be a region depleted of holes and containing uncovered bound negative charge, as indicated in Fig From the above it follows that a carrierdepletion region will exist on both sides of the junction, with the n side of this region positively charged and the p side negatively charged. This carrierdepletion region or, simply, depletion region is also called the spacecharge region. The charges on both sides of the depletion region cause an electric field E to be established across the region in the direction indicated in Fig Hence a potential difference results across the depletion region, with the n side at a positive voltage relative to the p side, as shown in Fig. 3.9(b). Thus the resulting electric field opposes the diffusion of holes into the n region and electrons into the p region. In fact, the voltage drop across the depletion region acts as a barrier that has to be overcome for holes to diffuse into the n region and electrons to diffuse into the p region. The larger the barrier voltage, the smaller the number of carriers that will be able to overcome the barrier, and hence the lower the magnitude of diffusion current. Thus it is the appearance of the barrier voltage V 0 that limits the carrier diffusion process. It follows that the diffusion current I D depends strongly on the voltage drop V 0 across the depletion region.
18 3.4 The pn Junction 151 The Drift Current I S and Equilibrium In addition to the current component I D due to majoritycarrier diffusion, a component due to minoritycarrier drift exists across the junction. Specifically, some of the thermally generated holes in the n material move toward the junction and reach the edge of the depletion region. There, they experience the electric field in the depletion region, which sweeps them across that region into the p side. Similarly, some of the minority thermally generated electrons in the p material move to the edge of the depletion region and get swept by the electric field in the depletion region across that region into the n side. These two current components electrons moved by drift from p to n and holes moved by drift from n to p add together to form the drift current I S, whose direction is from the n side to the p side of the junction, as indicated in Fig Since the current I S is carried by thermally generated minority carriers, its value is strongly dependent on temperature; however, it is independent of the value of the depletionlayer voltage V 0. This is due to the fact that the drift current is determined by the number of minority carriers that make it to the edge of the depletion region; any minority carriers that manage to get to the edge of the depletion region will be swept across by E irrespective of the value of E or, correspondingly, of V 0. Under opencircuit conditions (Fig. 3.9) no external current exists; thus the two opposite currents across the junction must be equal in magnitude: I D = I S This equilibrium condition 4 is maintained by the barrier voltage V 0. Thus, if for some reason I D exceeds I S, then more bound charge will be uncovered on both sides of the junction, the depletion layer will widen, and the voltage across it (V 0 ) will increase. This in turn causes I D to decrease until equilibrium is achieved with I D = I S. On the other hand, if I S exceeds I D, then the amount of uncovered charge will decrease, the depletion layer will narrow, and the voltage across it (V 0 ) will decrease. This causes I D to increase until equilibrium is achieved with I D = I S. The Junction Builtin Voltage With no external voltage applied, the barrier voltage V 0 across the pn junction can be shown to be given by 5 ( ) NA N V 0 = V T ln D (3.22) where N A and N D are the doping concentrations of the p side and n side of the junction, respectively. Thus V 0 depends both on doping concentrations and on temperature. It is known as the junction builtin voltage. Typically, for silicon at room temperature, V 0 is in the range of 0.6 V to 0.9 V. When the pn junction terminals are left opencircuited, the voltage measured between them will be zero. That is, the voltage V 0 across the depletion region does not appear between the junction terminals. This is because of the contact voltages existing at the metal semiconductor junctions at the terminals, which counter and exactly balance the barrier voltage. If this were not the case, we would have been able to draw energy from the isolated pn junction, which would clearly violate the principle of conservation of energy. Width of and Charge Stored in the Depletion Region Figure 3.10 provides further illustration of the situation that obtains in the pn junction when the junction is in equilibrium. n 2 i 4 In fact, in equilibrum the equality of drift and diffusion currents applies not just to the total currents but also to their individual components. That is, the hole drift current must equal the hole diffusion current and, similarly, the electron drift current must equal the electron diffusion current. 5 The derivation of this formula and of a number of others in this chapter can be found in textbooks dealing with devices, such as that by Streetman and Bannerjee (see the reading list in Appendix I).
19 152 Chapter 3 Semiconductors I D I S p x p 0 x n n E (a) p p N A n p0 n i 2 N A x p Carrier concentration 0 (b) W x n nn ND p n0 n i 2 N D x Charge density Q Aq N D x n x p x n x Q Aq N A x p W (c) Voltage V O x p 0 (d) x n Figure 3.10 (a) A pn junction with the terminals opencircuited. (b) Carrier concentrations; note that N A > N D. (c) The charge stored in both sides of the depletion region; Q J = Q+ = Q. (d) The builtin voltage V 0.
20 and that on the p side of the junction as Q = qaxp N A (3.24) 3.4 The pn Junction 153 In Fig. 3.10(a) we show a junction in which N A > N D, a typical situation in practice. This is borne out by the carrier concentration on both sides of the junction, as shown in Fig. 3.10(b). Note that we have denoted the minoritycarrier concentrations in both sides by n p0 and p n0, with the additional subscript 0 signifying equilibrium (i.e., before external voltages are applied, as will be seen in the next section). Observe that the depletion region extends in both the p and n materials and that equal amounts of charge exist on both sides (Q + and Q in Fig. 3.10c). However, since usually unequal dopings N A and N D are used, as in the case illustrated in Fig. 3.10, the width of the depletion layer will not be the same on the two sides. Rather, to uncover the same amount of charge, the depletion layer will extend deeper into the more lightly doped material. Specifically, if we denote the width of the depletion region in the p side by x p and in the n side by x n, we can express the magnitude of the charge on the n side of the junction as Q + = qax n N D (3.23) where A is the crosssectional area of the junction in the plane perpendicular to the page. The charge equality condition can now be written as which can be rearranged to yield qax n N D = qax p N A x n x p = N A N D (3.25) In actual practice, it is usual for one side of the junction to be much more heavily doped than the other, with the result that the depletion region exists almost entirely on one side (the lightly doped side). The width W of the depletion layer can be shown to be given by W = x n + x p = 2e s q ( N A N D ) V 0 (3.26) where e s is the electrical permittivity of silicon = 11.7e 0 = F/cm = F/cm. Typically W is in the range 0.1 μm to1μm. Eqs. (3.25) and (3.26) can be used to obtain x n and x p in terms of W as N A x n = W (3.27) N A + N D x p = W (3.28) N A + N D The charge stored on either side of the depletion region can be expressed in terms of W by utilizing Eqs. (3.23) and (3.27) to obtain Q J = Q + = Q ( ) NA N Q J = Aq D W (3.29) N A + N D Finally, we can substitute for W from Eq. (3.26) to obtain ( ) NA N Q J = A 2e s q D V N A + N 0 (3.30) D These expressions for Q J will prove useful in subsequent sections. N D
21 154 Chapter 3 Semiconductors Example 3.5 Consider a pn junction in equilibrium at room temperature (T = 300 K) for which the doping concentrations are N A = /cm 3 and N D = /cm 3 and the crosssectional area A = 10 4 cm 2. Calculate p p, n p0, n n, p n0, V 0, W, x n, x p, and Q J. Use n i = /cm 3. Solution To find V 0 we use Eq. (3.22), where Thus, p p N A = cm 3 n p0 = n2 i n2 i = ( ) = cm 3 p p N A n n N D = cm 3 p n0 = n2 i n2 i = ( ) = cm 3 n n N D ( ) NA N V O = V T ln D V T = kt q = (ev) q (e) = V ( ) V 0 = ln = V To determine W we use Eq. (3.26): ( W = ) n 2 i = cm = μm To determine x n and x p we use Eqs. (3.27) and (3.28), respectively: N A x n = W N A + N D = = μm N D x p = W N A + N D = = μm Finally, to determine the charge stored on either side of the depletion region, we use Eq. (3.29): ( ) Q J = = C = 5.18 pc
22 3.5 The pn Junction with an Applied Voltage 155 EXERCISES 3.7 Show that V 0 = 1 2 ( )( q NA N D e s N A + N D ) W Show that for a pn junction in which the p side is much more heavily doped than the n side (i.e., N A N D ), referred to as a p + n diode, Eqs. (3.26), (3.27), (3.28), (3.29), and (3.30) can be simplified as follows: 2e W s V qn 0 (3.26 ) D x n W (3.27 ) x p W/ ( ) N A /N D (3.28 ) Q J AqN D W (3.29 ) Q J A 2e s qn D V 0 (3.30 ) 3.9 If in the fabrication of the pn junction in Example 3.5, it is required to increase the minoritycarrier concentration in the n region by a factor of 2, what must be done? Ans. Lower N D by a factor of The pn Junction with an Applied Voltage Having studied the opencircuited pn junction in detail, we are now ready to apply a dc voltage between its two terminals to find its electrical conduction properties. If the voltage is applied so that the p side is made more positive than the n side, it is referred to as a forwardbias 6 voltage. Conversely, if our applied dc voltage is such that it makes the n side more positive than the p side, it is said to be a reversebias voltage. As will be seen, the pn junction exhibits vastly different conduction properties in its forward and reverse directions. Our plan is as follows. We begin by a simple qualitative description in Section and then consider an analytical description of the i v characteristic of the junction in Section Qualitative Description of Junction Operation Figure 3.11 shows the pn junction under three different conditions: (a) the opencircuit or equilibrium condition studied in the previous section; (b) the reversebias condition, where a dc voltage V R is applied; and (c) the forwardbias condition, where a dc voltage V F is applied. 6 For the time being, we take the term bias to refer simply to the application of a dc voltage. We will see in later chapters that it has a deeper meaning in the design of electronic circuits.
23 156 Chapter 3 Semiconductors V R V F I D I D I D I S I S I S p n p n p n V 0 (V 0 V R ) (V 0 V F ) (a) Opencircuit (equilibrium) (b) Reverse bias (c) Forward bias Figure 3.11 The pn junction in: (a) equilibrium; (b) reverse bias; (c) forward bias.
24 3.5 The pn Junction with an Applied Voltage 157 Observe that in the opencircuit case, a barrier voltage V 0 develops, making n more positive than p, and limiting the diffusion current I D to a value exactly equal to the drift current I S, thus resulting in a zero current at the junction terminals, as should be the case, since the terminals are opencircuited. Also, as mentioned previously, the barrier voltage V 0, though it establishes the current equilibrium across the junction, does not in fact appear between the junction terminals. Consider now the reversebias case in (b). The externally applied reversebias voltage V R is in the direction to add to the barrier voltage, and it does, thus increasing the effective barrier voltage to (V 0 + V R ) as shown. This reduces the number of holes that diffuse into the n region and the number of electrons that diffuse into the p region. The end result is that the diffusion current I D is dramatically reduced. As will be seen shortly, a reversebias voltage of a volt or so is sufficient to cause I D 0, and the current across the junction and through the external circuit will be equal to I S. Recalling that I S is the current due to the drift across the depletion region of the thermally generated minority carriers, we expect I S to be very small and to be strongly dependent on temperature. We will show this to be the case very shortly. We thus conclude that in the reverse direction, the pn junction conducts a very small and almostconstant current equal to I S. Before leaving the reversebias case, observe that the increase in barrier voltage will be accompanied by a corresponding increase in the stored uncovered charge on both sides of the depletion region. This in turn means a wider depletion region, needed to uncover the additional charge required to support the larger barrier voltage (V 0 + V R ). Analytically, these results can be obtained easily by a simple extension of the results of the equilibrium case. Thus the width of the depletion region can be obtained by replacing V 0 in Eq. (3.26) by (V 0 + V R ), W = x n + x p = ( 2e s ) (V q N A N 0 + V R ) (3.31) D and the magnitude of the charge stored on either side of the depletion region can be determined by replacing V 0 in Eq. (3.30) by (V 0 + V R ), ( ) NA N Q J = A 2e s q D (V N A + N 0 + V R ) (3.32) D We next consider the forwardbias case shown in Fig. 3.11(c). Here the applied voltage V F is in the direction that subtracts from the builtin voltage V 0, resulting in a reduced barrier voltage (V 0 V F ) across the depletion region. This reduced barrier voltage will be accompanied by reduced depletionregion charge and correspondingly narrower depletionregion width W. Most importantly, the lowering of the barrier voltage will enable more holes to diffuse from p to n and more electrons to diffuse from n to p. Thus the diffusion current I D increases substantially and, as will be seen shortly, can become many orders of magnitude larger than the drift current I S. The current I in the external circuit is of course the difference between I D and I S, I = I D I S and it flows in the forward direction of the junction, from p to n. We thus conclude that the pn junction can conduct a substantial current in the forwardbias region and that current is mostly a diffusion current whose value is determined by the forwardbias voltage V F.
25 158 Chapter 3 Semiconductors The Current Voltage Relationship of the Junction We are now ready to find an analytical expression that describes the current voltage relationship of the pn junction. In the following we consider a junction operating with a forward applied voltage V and derive an expression for the current I that flows in the forward direction (from p to n). However, our derivation is general and will be seen to yield the reverse current when the applied voltage V is made negative. From the qualitative description above we know that a forwardbias voltage V subtracts from the builtin voltage V 0, thus resulting in a lower barrier voltage (V 0 V). The lowered barrier in turn makes it possible for a greater number of holes to overcome the barrier and diffuse into the n region. A similar statement can be made about electrons from the n region diffusing into the p region. Let us now consider the holes injected into the n region. The concentration of holes in the n region at the edge of the depletion region will increase considerably. In fact, an important result from device physics shows that the steadystate concentration at the edge of the depletion region will be p n (x n ) = p n0 e V/V T (3.33) That is, the concentration of the minority holes increases from the equilibrium value of p n0 (see Fig. 3.10) to the much larger value determined by the value of V, given by Eq. (3.33). We describe this situation as follows: The forwardbias voltage V results in an excess concentration of minority holes at x = x n, given by Excess concentration = p n0 e V/V T p n0 ( V/V = p n0 e T 1 ) (3.34) The increase in minoritycarrier concentration in Eqs. (3.33) and (3.34) occurs at the edge of the depletion region (x = x n ). As the injected holes diffuse into the n material, some will recombine with the majority electrons and disappear. Thus, the excess hole concentration will decay exponentially with distance. As a result, the total hole concentration in the n material will be given by p n (x) = p n0 + (Excess concentration)e (x x n)/l p Substituting for the Excess concentration from Eq. (3.34) gives p n (x) = p n0 + p n0 ( e V/V T 1 ) e (x x n)/l p (3.35) The exponential decay is characterized by the constant L p, which is called the diffusion length of holes in the n material. The smaller the value of L p, the faster the injected holes will recombine with the majority electrons, resulting in a steeper decay of minoritycarrier concentration. Figure 3.12 shows the steadystate minoritycarrier concentration profiles on both sides of a pn junction in which N A N D. Let s stay a little longer with the diffusion of holes into the n region. Note that the shaded region under the exponential represents the excess minority carriers (holes). From our study of diffusion in Section 3.3, we know that the establishment of a carrier concentration profile such as that in Fig is essential to support a steadystate diffusion current. In fact, we can now find the value of the hole diffusion current density by applying Eq. (3.19), J p (x) = qd p dp n (x) dx
26 3.5 The pn Junction with an Applied Voltage 159 p n, n p p region Depletion region p n (x n ) n region Excess concentration p n (x) n p (x) n p (x p ) p n0 n p0 Thermal equilibrium value x p 0 x n x Figure 3.12 Minoritycarrier distribution in a forwardbiased pn junction. It is assumed that the p region is more heavily doped than the n region; N A N D. Substituting for p n (x) from Eq. (3.35) gives J p (x) = q ( Dp As expected, J p (x) is highest at x = x n, L p J p (x n ) = q ) p n0 ( e V/V T 1 ) e (x x n)/l p (3.36) ( Dp L p ) p n0 ( e V/V T 1 ) (3.37) and decays exponentially for x > x n, as the minority holes recombine with the majority electrons. This recombination, however, means that the majority electrons will have to be replenished by a current that injects electrons from the external circuit into the n region of the junction. This latter current component has the same direction as the hole current (because electrons moving from right to left give rise to current in the direction from left to right). It follows that as J p (x) decreases, the electron current component increases by exactly the same amount, making the total current in the n material constant at the value given by Eq. (3.37). An exactly parallel development can be applied to the electrons that are injected from the n to the p region, resulting in an electron diffusion current given by a simple adaptation of Eq. (3.37), ( ) ( ) Dn ( V/V J n xp = q n L p0 e T 1 ) (3.38) n Now, although the currents in Eqs. (3.37) and (3.38) are found at the two edges of the depletion region, their values do not change in the depletion region. Thus we can drop the location descriptors (x n ), ( x p ), add the two current densities, and multiply by the junction area A to
27 160 Chapter 3 Semiconductors obtain the total current I as I = A ( J p + J n ) I = Aq ( Dp p L n0 + D ) n (e V/V n T p L p0 1 ) n Substituting for p n0 = n 2 i /N D and for n p0 = n 2 i /N A gives I = Aqn 2 i ( Dp + D ) n (e V/V T 1 ) (3.39) L p N D L n N A From this equation we note that for a negative V (reverse bias) with a magnitude of a few times V T (25.9 mv), the exponential term becomes essentially zero, and the current across the junction becomes negative and constant. From our qualitative description in Section 3.5.1, we know that this current must be I S. Thus, I = I S ( e V/V T 1 ) (3.40) where I S = Aqn 2 i ( Dp + D ) n L p N D L n N A (3.41) Figure 3.13 shows the I V characteristic of the pn junction (Eq. 3.40). Observe that in the reverse direction the current saturates at a value equal to I S. For this reason, I S is given the name saturation current. From Eq. (3.41) we see that I S is directly proportional to the crosssectional area A of the junction. Thus, another name for I S, one we prefer to use in this book, is the junction scale current. Typical values for I S, for junctions of various areas, range from Ato10 12 A. Besides being proportional to the junction area A, the expression for I S in Eq. (3.41) indicates that I S is proportional to n 2 i, which is a very strong function of temperature (see Eq. 3.2). I 0 I S 0 V Figure 3.13 The pn junction I V characteristic.
28 3.5 The pn Junction with an Applied Voltage 161 Example 3.6 For the pn junction considered in Example 3.5 for which N A =10 18 /cm 3, N D =10 16 /cm 3, A=10 4 cm 2, and n i = /cm 3, let L p = 5 μm, L n = 10 μm, D p (in the n region) = 10 cm 2 /V s, and D n (in the p region) = 18 cm 2 /V s. The pn junction is forward biased and conducting a current I = 0.1 ma. Calculate: (a) I S ; (b) the forwardbias voltage V; and (c) the component of the current I due to hole injection and that due to electron injection across the junction. Solution (a) Using Eq. (3.41), we find I S as I S = ( ) 2 ( ) (b) In the forward direction, Thus, For I = 0.1 ma, = A I = I S ( e V/V T 1 ) I S e V/V T ( ) I V = V T ln I S ( ) V = ln = V (c) The holeinjection component of I can be found using Eq. (3.37) I p = Aq D p ( V/V p L n0 e T 1 ) p Similarly, I n can be found using Eq. (3.39), Thus, For our case, = Aq D p n 2 ( i V/V e T 1 ) L p N D I n = Aq D n n 2 ( i V/V e T 1 ) L n N A I p I n = ( )( )( Dp Ln NA D n L p N D I p I n = = = 111 )
29 162 Chapter 3 Semiconductors Example 3.6 continued Thus most of the current is conducted by holes injected into the n region. Specifically, I p = = ma 112 I n = = ma 112 This stands to reason, since the p material has a doping concentration 100 times that of the n material. EXERCISES 3.10 Show that if N A N D, D I S Aqn 2 p i L p N D 3.11 For the pn junction in Example 3.6, find the value of I S and that of the current I at V = V (same voltage found in Example 3.6 at a current I = 0.1 ma) if N D is reduced by a factor of 2. Ans A; 0.2 ma 3.12 For the pn junction considered in Examples 3.5 and 3.6, find the width of the depletion region W corresponding to the forwardbias voltage found in Example 3.6. (Hint: Use the formula in Eq. (3.31) with V R replaced with V F.) Ans μm 3.13 For the pn junction considered in Examples 3.5 and 3.6, find the width of the depletion region W and the charge stored in the depletion region Q J when a 2V reverse bias is applied. Also find the value of the reverse current I. Ans μm; 9.63 pc; A Reverse Breakdown The description of the operation of the pn junction in the reverse direction, and the I V relationship of the junction in Eq. (3.40), indicate that at a reversebias voltage V, with V V T, the reverse current that flows across the junction is approximately equal to I S and thus is very small. However, as the magnitude of the reversebias voltage V is increased, a value is reached at which a very large reverse current flows as shown in Fig Observe that as V reaches the value V Z, the dramatic increase in reverse current is accompanied by a very small increase in the reverse voltage; that is, the reverse voltage across the junction
30 3.5 The pn Junction with an Applied Voltage 163 I V Z 0 V Figure 3.14 The I V characteristic of the pn junction showing the rapid increase in reverse current in the breakdown region. remains very close to the value V Z. The phenomenon that occurs at V = V Z is known as junction breakdown. It is not a destructive phenomenon. That is, the pn junction can be repeatedly operated in the breakdown region without a permanent effect on its characteristics. This, however, is predicated on the assumption that the magnitude of the reversebreakdown current is limited by the external circuit to a safe value. The safe value is one that results in the limitation of the power dissipated in the junction to a safe, allowable level. There are two possible mechanisms for pn junction breakdown: the zener effect 7 and the avalanche effect. Ifapn junction breaks down with a breakdown voltage V Z < 5V,the breakdown mechanism is usually the zener effect. Avalanche breakdown occurs when V Z is greater than approximately 7 V. For junctions that break down between 5 V and 7 V, the breakdown mechanism can be either the zener or the avalanche effect or a combination of the two. Zener breakdown occurs when the electric field in the depletion layer increases to the point of breaking covalent bonds and generating electron hole pairs. The electrons generated in this way will be swept by the electric field into the n side and the holes into the p side. Thus these electrons and holes constitute a reverse current across the junction. Once the zener effect starts, a large number of carriers can be generated, with a negligible increase in the junction voltage. Thus the reverse current in the breakdown region will be large and its value must be determined by the external circuit, while the reverse voltage appearing between the diode terminals will remain close to the specified breakdown voltage V Z. The other breakdown mechanism, avalanche breakdown, occurs when the minority carriers that cross the depletion region under the influence of the electric field gain sufficient kinetic energy to be able to break covalent bonds in atoms with which they collide. The carriers liberated by this process may have sufficiently high energy to be able to cause other carriers to be liberated in another ionizing collision. This process keeps repeating in the fashion of an avalanche, with the result that many carriers are created that are able to support any value of 7 Named after an early worker in the area. Note that the subscript Z in V Z denotes zener. We will use V Z to denote the breakdown voltage whether the breakdown mechanism is the zener effect or the avalanche effect.
31 164 Chapter 3 Semiconductors reverse current, as determined by the external circuit, with a negligible change in the voltage drop across the junction. As will be seen in Chapter 4, some pn junction diodes are fabricated to operate specifically in the breakdown region, where use is made of the nearly constant voltage V Z. 3.6 Capacitive Effects in the pn Junction There are two chargestorage mechanisms in the pn junction. One is associated with the charge stored in the depletion region, and the other is associated with the minoritycarrier charge stored in the n and p materials as a result of the concentration profiles established by carrier injection. While the first is easier to see when the pn junction is reverse biased, the second is in effect only when the junction is forward biased Depletion or Junction Capacitance When a pn junction is reverse biased with a voltage V R, the charge stored on either side of the depletion region is given by Eq. (3.32), Thus, for a given pn junction, Q J = A 2e s q N AN D N A + N D (V 0 + V R ) Q J = α V 0 + V R (3.42) where α is given by α = A 2e s q N AN D N A + N D (3.43) Thus Q J is nonlinearly related to V R, as shown in Fig This nonlinear relationship makes it difficult to define a capacitance that accounts for the need to change Q J whenever V R is Charge stored in depletion layer, Q J Slope C J Q Bias point 0 V Q Reverse voltage,v R Figure 3.15 The charge stored on either side of the depletion layer as a function of the reverse voltage V R.
32 3.6 Capacitive Effects in the pn Junction 165 changed. We can, however, assume that the junction is operating at a point such as Q, as indicated in Fig. 3.15, and define a capacitance C j that relates the change in the charge Q J to a change in the voltage V R, C j = dq J (3.44) dv R V R =V Q This incrementalcapacitance approach turns out to be quite useful in electronic circuit design, as we shall see throughout this book. Using Eq. (3.44) together with Eq. (3.42) yields C j = α 2 V 0 + V R (3.45) The value of C j at zero reverse bias can be obtained from Eq. (3.45) as which enables us to express C j as C j0 = α 2 V 0 (3.46) C j = C j0 1 + V R V 0 (3.47) where C j0 is given by Eq. (3.46) or alternatively if we substitute for α from Eq. (3.43) by (es q ) ( )( ) N C j0 = A A N D 1 2 N A + N D V 0 (3.48) Before leaving the subject of depletionregion or junction capacitance we point out that in the pn junction we have been studying, the doping concentration is made to change abruptly at the junction boundary. Such a junction is known as an abrupt junction. There is another type of pn junction in which the carrier concentration is made to change gradually from one side of the junction to the other. To allow for such a graded junction, the formula for the junction capacitance (Eq. 3.47) can be written in the more general form C j0 C j = ( 1 + V ) m (3.49) R V 0 where m is a constant called the grading coefficient, whose value ranges from 1/3 to 1/2 depending on the manner in which the concentration changes from the p to the n side.
33 166 Chapter 3 Semiconductors EXERCISE 3.14 For the pn junction considered in Examples 3.5 and 3.6, find C j0 and C j at V R = 2 V. Recall that V 0 = V, N A = /cm 3, N D = /cm 3, and A = 10 4 cm 2. Ans. 3.2 pf; 1.7 pf Diffusion Capacitance Consider a forwardbiased pn junction. In steady state, minoritycarrier distributions in the p and n materials are established, as shown in Fig Thus a certain amount of excess minoritycarrier charge is stored in each of the p and n bulk regions (outside the depletion region). If the terminal voltage V changes, this charge will have to change before a new steady state is achieved. This chargestorage phenomenon gives rise to another capacitive effect, distinctly different from that due to charge storage in the depletion region. To calculate the excess minoritycarrier charge, refer to Fig The excess hole charge stored in the n region can be found from the shaded area under the exponential as follows: 8 Q p = Aq shaded area under the p n (x)curve = Aq[p n (x n ) p n0 ]L p Substituting for p n (x n ) from Eq. (3.33) and using Eq. (3.37) enables us to express Q p as Q p = L2 p D p I p (3.50) The factor ( L 2 p/d p ) that relates Qp to I p is a useful device parameter that has the dimension of time (s) and is denoted τ p Thus, τ p = L2 p D p (3.51) Q p = τ p I p (3.52) The time constant τ p is known as the excess minoritycarrier (hole) lifetime. It is the average time it takes for a hole injected into the n region to recombine with a majority electron. This definition of τ p implies that the entire charge Q p disappears and has to be replenished every τ p seconds. The current that accomplishes the replenishing is I p = Q p /τ p. This is an alternate derivation for Eq. (3.52). 8 Recall that the area under an exponential curve Ae x/b is equal to AB.
34 3.6 Capacitive Effects in the pn Junction 167 A relationship similar to that in Eq. (3.52) can be developed for the electron charge stored in the p region, Q n = τ n I n (3.53) where τ n is the electron lifetime in the p region. The total excess minoritycarrier charge can be obtained by adding together Q p and Q n, Q = τ p I p + τ n I n (3.54) This charge can be expressed in terms of the diode current I = I p + I n as Q = τ T I (3.55) where τ T is called the mean transit time of the junction. Obviously, τ T is related to τ p and τ n. Furthermore, for most practical devices, one side of the junction is much more heavily doped than the other. For instance, if N A N D, one can show that I p I n, I I p, Q p Q n, Q Q p, and thus τ T τ p. For small changes around a bias point, we can define an incremental diffusion capacitance C d as C d = dq dv (3.56) and can show that ( ) τt C d = I (3.57) V T where I is the forwardbias current. Note that C d is directly proportional to the forward current I and thus is negligibly small when the diode is reverse biased. Also note that to keep C d small, the transit time τ T must be made small, an important requirement for a pn junction intended for highspeed or highfrequency operation. EXERCISES 3.15 Use the definition of C d in Eq. (3.56) to derive the expression in Eq. (3.57) by means of Eqs. (3.55) and (3.40) For the pn junction considered in Examples 3.5 and 3.6 for which D p = 10 cm 2 /V s, and L p = 5 μm, find τ p and C d at a forwardbias current of 0.1 ma. Recall that for this junction, I p I. Ans. 25 ns; 96.5 pf
35 168 Chapter 3 Semiconductors Summary Today s microelectronics technology is almost entirely based on the semiconductor material silicon. If a circuit is to be fabricated as a monolithic integrated circuit (IC) it is made using a single silicon crystal, no matter how large the circuit is (a recent chip contains 4.31 billion transistors). In a crystal of intrinsic or pure silicon, the atoms are held in position by covalent bonds. At very low temperatures, all the bonds are intact, and no charge carriers are available to conduct electrical current. Thus, at such low temperatures, silicon behaves as an insulator. At room temperature, thermal energy causes some of the covalent bonds to break, thus generating free electrons and holes that become available for current conduction. Current in semiconductors is carried by free electrons and holes. Their numbers are equal and relatively small in intrinsic silicon. The conductivity of silicon can be increased dramatically by introducing small amounts of appropriate impurity materials into the silicon crystal in a process called doping. There are two kinds of doped semiconductor: ntype, in which electrons are abundant, and ptype, in which holes are abundant. There are two mechanisms for the transport of charge carriers in semiconductors: drift and diffusion. Carrier drift results when an electric field E is applied across a piece of silicon. The electric field accelerates the holes in the direction of E and the electrons in the direction opposite to E. These two current components add together to produce a drift current in the direction of E. Carrier diffusion occurs when the concentration of charge carriers is made higher in one part of the silicon crystal than in other parts. To establish a steadystate diffusion current, a carrier concentration gradient must be maintained in the silicon crystal. A basic semiconductor structure is the pn junction. It is fabricated in a silicon crystal by creating a p region in close proximity to an n region. The pn junction is a diode and plays a dominant role in the structure and operation of transistors. When the terminals of the pn junction are left open, no current flows externally. However, two equal and opposite currents, I D and I S, flow across the junction, and equilibrium is maintained by a builtin voltage V 0 that develops across the junction, with the n side positive relative to the p side. Note, however, that the voltage across an open junction is 0 V, since V 0 is canceled by potentials appearing at the metaltosemiconductor connection interfaces. The voltage V 0 appears across the depletion region, which extends on both sides of the junction. The diffusion current I D is carried by holes diffusing from p to n and electrons diffusing from n to p. I D flows from p to n, which is the forward direction of the junction. Its value depends on V 0. The drift current I S is carried by thermally generated minority electrons in the p material that are swept across the depletion layer into the n side, and by thermally generated minority holes in the n side that are swept across the depletion region into the p side. I S flows from n to p, in the reverse direction of the junction, and its value is a strong function of temperature but independent of V 0. Forward biasing the pn junction, that is, applying an external voltage V that makes p more positive than n, reduces the barrier voltage to V 0 V and results in an exponential increase in I D while I S remains unchanged. The net result is a substantial current I = I D I S that flows across the junction and through the external circuit. Applying a negative V reverse biases the junction and increases the barrier voltage, with the result that I D is reduced to almost zero and the net current across the junction becomes the very small reverse current I S. If the reverse voltage is increased in magnitude to a value V Z specific to the particular junction, the junction breaks down, and a large reverse current flows. The value of the reverse current must be limited by the external circuit. Whenever the voltage across a pn junction is changed, some time has to pass before steady state is reached. This is due to the chargestorage effects in the junction, which are modeled by two capacitances: the junction capacitance C j and the diffusion capacitance C d. For future reference, we present in Table 3.1 a summary of pertinent relationships and the values of physical constants.
36 Summary 169 Table 3.1 Summary of Important Equations Values of Constants and Parameters Quantity Relationship (for Intrinsic Si at T = 300 K) Carrier concentration in intrinsic silicon (cm 3 ) n i = BT 3/2 e E g /2kT B= cm 3 K 3/2 E g = 1.12 ev k = ev/k n i = /cm 3 Diffusion current density (A/cm 2 ) J p = qd p dp dx J n = qd n dn dx q= coulomb D p = 12 cm 2 /s D n = 34 cm 2 /s Drift current density (A/cm 2 ) J drift = q ( pμ p + nμ n ) E μp = 480 cm 2 /V s μ n = 1350 cm 2 /V s Resistivity ( cm) ρ = 1/ [ q ( pμ p + nμ n )] μ p and μ n decrease with the increase in doping concentration Relationship between mobility and diffusivity D n μ n = D p μ p = V T V T = kt/q 25.9 mv Carrier concentration in ntype silicon (cm 3 ) n n0 N D p n0 = n 2 i /N D Carrier concentration in ptype silicon (cm 3 ) p p0 N A n p0 = n 2 i /N A Junction builtin ( ) NA N voltage (V) V 0 = V T ln D n 2 i Width of depletion region (cm) x n = N A x p N D W = x n + x p = 2e s q ( 1 N A + 1 N D ) (V0 + V R ) e s = 11.7e 0 e 0 = F/cm
37 170 Chapter 3 Semiconductors Table 3.1 continued Values of Constants and Parameters Quantity Relationship (for Intrinsic Si at T = 300 K) Charge stored in depletion layer (coulomb) Q J = q N A N D N A + N D AW Forward current (A) I = I p + I n D ( ) I p = Aqn 2 p i e V/V T 1 L p N D I n = Aqn 2 i D ( ) n e V/V T 1 L n N A Saturation current (A) I S = Aqn 2 i ( Dp D n + L p N D L n N A ) ) I V relationship I = I S (e V/V T 1 Minoritycarrier lifetime (s) τ p = L 2 p /D p τ n = L 2 n /D n L p,l n = 1 μm to 100 μm τ p,τ n = 1nsto10 4 ns Minoritycarrier charge storage (coulomb) Q p = τ p I p Q n = τ n I n Q= Q p + Q n = τ T I Depletion capacitance (F) ( es q ) ( ) N C j0 = A A N D 1 2 N A + N D V 0 /( C j = C j0 1 + V ) m R V 0 m = 1 3 to 1 2 Diffusion capacitance (F) ( ) τt C d = I V T
38 PROBLEMS If in the following problems the need arises for the values of particular parameters or physical constants that are not stated, please consult Table 3.1. Section 3.1: Intrinsic Semiconductors 3.1 Find values of the intrinsic carrier concentration n i for silicon at 55 C, 0 C, 20 C, 75 C, and 125 C. At each temperature, what fraction of the atoms is ionized? Recall that a silicon crystal has approximately atoms/cm Calculate the value of n i for gallium arsenide (GaAs) at T = 300 K. The constant B = cm 3 K 3/2 and the bandgap voltage E g = 1.42 ev. Section 3.2: Doped Semiconductors 3.3 For a ptype silicon in which the dopant concentration N A = /cm 3, find the hole and electron concentrations at T = 300 K. 3.4 For a silicon crystal doped with phosphorus, what must N D be if at T = 300 K the hole concentration drops below the intrinsic level by a factor of 10 8? 3.5 In a phosphorusdoped silicon layer with impurity concentration of /cm 3, find the hole and electron concentrations at 27 C and 125 C. of 3 V is imposed. Let μ n = 1350 cm 2 /V s and μ p = 480 cm 2 /V s 3.8 Find the current that flows in a silicon bar of 10μm length having a 5μm 4μm crosssection and having freeelectron and hole densities of 10 4 /cm 3 and /cm 3, respectively, when a 1 V is applied endtoend. Use μ n = 1200 cm 2 /V s and μ p = 500 cm 2 /V s. 3.9 In a 10μmlong bar of donordoped silicon, what donor concentration is needed to realize a current density of 2 ma/μm 2 in response to an applied voltage of 1 V? (Note: Although the carrier mobilities change with doping concentration, as a first approximation you may assume μ n to be constant and use 1350 cm 2 /V s, the value for intrinsic silicon.) 3.10 Holes are being steadily injected into a region of ntype silicon (connected to other devices, the details of which are not important for this question). In the steady state, the excesshole concentration profile shown in Fig. P3.10 is established in the ntype silicon region. Here excess means over and above the thermalequilibrium concentration (in the absence of hole injection), denoted p n0.ifn D = /cm 3, n i = /cm 3, D p = 12 cm 2 /s, and W = 50 nm, find the density of the current that will flow in the x direction. Section 3.3: Current Flow in Semiconductors 3.6 A young designer, aiming to develop intuition concerning conducting paths within an integrated circuit, examines the endtoend resistance of a connecting bar 10μm long, 3μm wide, and 1 μm thick, made of various materials. The designer considers: 10 8 p n0 p n0 p n (x) n region (a) intrinsic silicon (b) ndoped silicon with N D = /cm 3 (c) ndoped silicon with N D = /cm 3 (d) pdoped silicon with N A = /cm 3 (e) aluminum with resistivity of 2.8 μ cm Figure P W x Find the resistance in each case. For intrinsic silicon, use the data in Table 3.1. For doped silicon, assume μ n = 3μ p = 1200 cm 2 /V s. (Recall that R = ρl/a.) 3.7 Contrast the electron and hole drift velocities through a 10μm layer of intrinsic silicon across which a voltage 3.11 Both the carrier mobility and the diffusivity decrease as the doping concentration of silicon is increased. Table P3.11 provides a few data points for μ n and μ p versus doping concentration. Use the Einstein relationship to obtain the corresponding values for D n and D p. = Multisim/PSpice; * = difficult problem; ** = more difficult; *** = very challenging; D = design problem
Diodes. anode. cathode. cutoff. Can be approximated by a piecewiselinearlike characteristic. Lecture 91
Diodes mplest nonlinear circuit element Basic operation sets the foundation for Bipolar Junction Transistors (BJTs) Also present in Field Effect Transistors (FETs) Ideal diode characteristic anode cathode
More informationBasic Physics of Semiconductors
Basic Physics of Semiconductors Semiconductor materials and their properties PNjunction diodes Reverse Breakdown EEM 205 Electronics I Dicle University, EEE Dr. Mehmet Siraç ÖZERDEM Semiconductor Physics
More informationSEMICONDUCTORS. Conductivity lies between conductors and insulators. The flow of charge in a metal results from the
SEMICONDUCTORS Conductivity lies between conductors and insulators The flow of charge in a metal results from the movement of electrons Electros are negatively charged particles (q=1.60x1019 C ) The outermost
More informationEE301 Electronics I , Fall
EE301 Electronics I 20182019, Fall 1. Introduction to Microelectronics (1 Week/3 Hrs.) Introduction, Historical Background, Basic Consepts 2. Rewiev of Semiconductors (1 Week/3 Hrs.) Semiconductor materials
More informationECE 142: Electronic Circuits Lecture 3: Semiconductors
Faculty of Engineering ECE 142: Electronic Circuits Lecture 3: Semiconductors Agenda Intrinsic Semiconductors Extrinsic Semiconductors Ntype Ptype Carrier Transport Drift Diffusion Semiconductors A semiconductor
More informationElectro  Principles I
Electro  Principles I Page 101 Atomic Theory It is necessary to know what goes on at the atomic level of a semiconductor so the characteristics of the semiconductor can be understood. In many cases a
More informationChapter 1 Semiconductor basics
Chapter 1 Semiconductor basics ELECH402/CH1: Semiconductor basics 1 Basic semiconductor concepts Semiconductor basics Semiconductors, silicon and holeelectron pair Intrinsic silicon properties Doped
More informationITT Technical Institute ET215 Devices I Unit 1
ITT Technical Institute ET215 Devices I Unit 1 Chapter 1 Chapter 2, Sections 2.12.4 Chapter 1 Basic Concepts of Analog Circuits Recall ET115 & ET145 Ohms Law I = V/R If voltage across a resistor increases
More informationECE 250 Electronic Devices 1. Electronic Device Modeling
ECE 250 Electronic Devices 1 ECE 250 Electronic Device Modeling ECE 250 Electronic Devices 2 Introduction to Semiconductor Physics You should really take a semiconductor device physics course. We can only
More informationChapter 2. Electronics I  Semiconductors
Chapter 2 Electronics I  Semiconductors Fall 2017 talarico@gonzaga.edu 1 Charged Particles The operation of all electronic devices is based on controlling the flow of charged particles There are two type
More informationLecture (02) Introduction to Electronics II, PN Junction and Diodes I
Lecture (02) Introduction to Electronics II, PN Junction and Diodes I By: Dr. Ahmed ElShafee ١ Agenda Current in semiconductors/conductors N type, P type semiconductors N Type Semiconductor P Type Semiconductor
More informationcollisions of electrons. In semiconductor, in certain temperature ranges the conductivity increases rapidly by increasing temperature
1.9. Temperature Dependence of Semiconductor Conductivity Such dependence is one most important in semiconductor. In metals, Conductivity decreases by increasing temperature due to greater frequency of
More informationELECTRONIC I Lecture 1 Introduction to semiconductor. By Asst. Prof Dr. Jassim K. Hmood
ELECTRONIC I Lecture 1 Introduction to semiconductor By Asst. Prof Dr. Jassim K. Hmood SOLIDSTATE ELECTRONIC MATERIALS Electronic materials generally can be divided into three categories: insulators,
More informationAtoms? All matters on earth made of atoms (made up of elements or combination of elements).
Chapter 1 Atoms? All matters on earth made of atoms (made up of elements or combination of elements). Atomic Structure Atom is the smallest particle of an element that can exist in a stable or independent
More informationDiodes. EE223 Digital & Analogue Electronics Derek Molloy 2012/2013.
Diodes EE223 Digital & Analogue Electronics Derek Molloy 2012/2013 Derek.Molloy@dcu.ie Diodes: A Semiconductor? Conductors Such as copper, aluminium have a cloud of free electrons weak bound valence electrons
More informationJunction Diodes. Tim Sumner, Imperial College, Rm: 1009, x /18/2006
Junction Diodes Most elementary solid state junction electronic devices. They conduct in one direction (almost correct). Useful when one converts from AC to DC (rectifier). But today diodes have a wide
More informationLecture (02) PN Junctions and Diodes
Lecture (02) PN Junctions and Diodes By: Dr. Ahmed ElShafee ١ I Agenda N type, P type semiconductors N Type Semiconductor P Type Semiconductor PN junction Energy Diagrams of the PN Junction and Depletion
More informationEngineering 2000 Chapter 8 Semiconductors. ENG2000: R.I. Hornsey Semi: 1
Engineering 2000 Chapter 8 Semiconductors ENG2000: R.I. Hornsey Semi: 1 Overview We need to know the electrical properties of Si To do this, we must also draw on some of the physical properties and we
More informationLecture 0. EE206 Electronics I
Lecture 0 Course Overview EE206 Electronics I Course description: Theory, characteristics and operation of diodes, bipolar junction transistors and MOSFET transistors. When: Tue Thu 10:3012:20 (Lectures)
More informationELECTRONIC DEVICES AND CIRCUITS SUMMARY
ELECTRONIC DEVICES AND CIRCUITS SUMMARY Classification of Materials: Insulator: An insulator is a material that offers a very low level (or negligible) of conductivity when voltage is applied. Eg: Paper,
More informationCharge Carriers in Semiconductor
Charge Carriers in Semiconductor To understand PN junction s IV characteristics, it is important to understand charge carriers behavior in solids, how to modify carrier densities, and different mechanisms
More information16EC401 BASIC ELECTRONIC DEVICES UNIT I PN JUNCTION DIODE. Energy Band Diagram of Conductor, Insulator and Semiconductor:
16EC401 BASIC ELECTRONIC DEVICES UNIT I PN JUNCTION DIODE Energy bands in Intrinsic and Extrinsic silicon: Energy Band Diagram of Conductor, Insulator and Semiconductor: 1 2 Carrier transport: Any motion
More informationECE342 Test 2 Solutions, Nov 4, :008:00pm, Closed Book (one page of notes allowed)
ECE342 Test 2 Solutions, Nov 4, 2008 6:008:00pm, Closed Book (one page of notes allowed) Please use the following physical constants in your calculations: Boltzmann s Constant: Electron Charge: Free
More informationSemiconductor physics I. The Crystal Structure of Solids
Lecture 3 Semiconductor physics I The Crystal Structure of Solids 1 Semiconductor materials Types of solids Space lattices Atomic Bonding Imperfection and doping in SOLIDS 2 Semiconductor Semiconductors
More informationChapter 1 Overview of Semiconductor Materials and Physics
Chapter 1 Overview of Semiconductor Materials and Physics Professor Paul K. Chu Conductivity / Resistivity of Insulators, Semiconductors, and Conductors Semiconductor Elements Period II III IV V VI 2 B
More informationSemiconductor Physics Problems 2015
Semiconductor Physics Problems 2015 Page and figure numbers refer to Semiconductor Devices Physics and Technology, 3rd edition, by SM Sze and MK Lee 1. The purest semiconductor crystals it is possible
More informationElectronic PRINCIPLES
MALVINO & BATES Electronic PRINCIPLES SEVENTH EDITION Chapter 2 Semiconductors Topics Covered in Chapter 2 Conductors Semiconductors Silicon crystals Intrinsic semiconductors Two types of flow Doping a
More informationDetermination of properties in semiconductor materials by applying Matlab
Determination of properties in semiconductor materials by applying Matlab Carlos Figueroa. 1, Raúl Riera A. 2 1 Departamento de Ingeniería Industrial. Universidad de Sonora A.P. 5088, Hermosillo, Sonora.
More informationLecture 2. Semiconductor Physics. Sunday 4/10/2015 Semiconductor Physics 11
Lecture 2 Semiconductor Physics Sunday 4/10/2015 Semiconductor Physics 11 Outline Intrinsic bond model: electrons and holes Charge carrier generation and recombination Intrinsic semiconductor Doping:
More informationConcept of Core IENGINEERS CONSULTANTS LECTURE NOTES SERIES ELECTRONICS ENGINEERING 1 YEAR UPTU. Page 1
Concept of Core Conductivity of conductor and semiconductor can also be explained by concept of Core. Core: Core is a part of an atom other than its valence electrons. Core consists of all inner shells
More informationECE PN Junctions and Diodes
ECE 342 2. PN Junctions and iodes Jose E. SchuttAine Electrical & Computer Engineering University of Illinois jschutt@emlab.uiuc.edu ECE 342 Jose Schutt Aine 1 B: material dependent parameter = 5.4 10
More informationQuiz #1 Practice Problem Set
Name: Student Number: ELEC 3908 Physical Electronics Quiz #1 Practice Problem Set? Minutes January 22, 2016  No aids except a nonprogrammable calculator  All questions must be answered  All questions
More informationLecture 1. OUTLINE Basic Semiconductor Physics. Reading: Chapter 2.1. Semiconductors Intrinsic (undoped) silicon Doping Carrier concentrations
Lecture 1 OUTLINE Basic Semiconductor Physics Semiconductors Intrinsic (undoped) silicon Doping Carrier concentrations Reading: Chapter 2.1 EE105 Fall 2007 Lecture 1, Slide 1 What is a Semiconductor? Low
More informationUnit IV Semiconductors Engineering Physics
Introduction A semiconductor is a material that has a resistivity lies between that of a conductor and an insulator. The conductivity of a semiconductor material can be varied under an external electrical
More information3C3 Analogue Circuits
Department of Electronic & Electrical Engineering Trinity College Dublin, 2014 3C3 Analogue Circuits Prof J K Vij jvij@tcd.ie Lecture 1: Introduction/ Semiconductors & Doping 1 Course Outline (subject
More informationIntroduction to Semiconductor Physics. Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India
Introduction to Semiconductor Physics 1 Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India http://folk.uio.no/ravi/cmp2013 Review of Semiconductor Physics Semiconductor fundamentals
More informationEE 446/646 Photovoltaic Devices I. Y. Baghzouz
EE 446/646 Photovoltaic Devices I Y. Baghzouz What is Photovoltaics? First used in about 1890, the word has two parts: photo, derived from the Greek word for light, volt, relating to electricity pioneer
More informationLecture 3 Semiconductor Physics (II) Carrier Transport
Lecture 3 Semiconductor Physics (II) Carrier Transport Thermal Motion Carrier Drift Carrier Diffusion Outline Reading Assignment: Howe and Sodini; Chapter 2, Sect. 2.42.6 6.012 Spring 2009 Lecture 3 1
More informationElectronic Circuits for Mechatronics ELCT 609 Lecture 2: PN Junctions (1)
Electronic Circuits for Mechatronics ELCT 609 Lecture 2: PN Junctions (1) Assistant Professor Office: C3.315 Email: eman.azab@guc.edu.eg 1 Electronic (Semiconductor) Devices PN Junctions (Diodes): Physical
More informationKATIHAL FİZİĞİ MNT510
KATIHAL FİZİĞİ MNT510 YARIİLETKENLER Kaynaklar: Katıhal Fiziği, Prof. Dr. Mustafa Dikici, Seçkin Yayıncılık Katıhal Fiziği, Şakir Aydoğan, Nobel Yayıncılık, Physics for Computer Science Students: With
More informationElectronics EC /2/2012. * Inclass exams: 40% 7 th week exam 25% 12 th week exam 15%
Arab Academy for Science, Technology and Maritime Transport Electronics EC 331 Dr. Mohamed Hassan Course Assessment * Inclass exams: 40% 7 th week exam 25% 12 th week exam 15% *Tutorial exams and activities:
More information1 Name: Student number: DEPARTMENT OF PHYSICS AND PHYSICAL OCEANOGRAPHY MEMORIAL UNIVERSITY OF NEWFOUNDLAND. Fall :0011:00
1 Name: DEPARTMENT OF PHYSICS AND PHYSICAL OCEANOGRAPHY MEMORIAL UNIVERSITY OF NEWFOUNDLAND Final Exam Physics 3000 December 11, 2012 Fall 2012 9:0011:00 INSTRUCTIONS: 1. Answer all seven (7) questions.
More informationSemiconductor Physics fall 2012 problems
Semiconductor Physics fall 2012 problems 1. An ntype sample of silicon has a uniform density N D = 10 16 atoms cm 3 of arsenic, and a ptype silicon sample has N A = 10 15 atoms cm 3 of boron. For each
More informationLecture4 Junction Diode Characteristics
1 Lecture4 Junction Diode Characteristics PartII Q: Aluminum is alloyed into ntype Si sample (N D = 10 16 cm 3 ) forming an abrupt junction of circular crosssection, with an diameter of 0.02 in. Assume
More informationSection 12: Intro to Devices
Section 12: Intro to Devices Extensive reading materials on reserve, including Robert F. Pierret, Semiconductor Device Fundamentals Bond Model of Electrons and Holes Si Si Si Si Si Si Si Si Si Silicon
More informationCLASS 12th. Semiconductors
CLASS 12th Semiconductors 01. Distinction Between Metals, Insulators and SemiConductors Metals are good conductors of electricity, insulators do not conduct electricity, while the semiconductors have
More informationn N D n p = n i p N A
Summary of electron and hole concentration in semiconductors Intrinsic semiconductor: E G n kt i = pi = N e 2 0 Donordoped semiconductor: n N D where N D is the concentration of donor impurity Acceptordoped
More informationelectronics fundamentals
electronics fundamentals circuits, devices, and applications THOMAS L. FLOYD DAVID M. BUCHLA Lesson 1: Diodes and Applications Semiconductors Figure 11 The Bohr model of an atom showing electrons in orbits
More informationPN Junction
P Junction 20170504 Definition Power Electronics = semiconductor switches are used Analogue amplifier = high power loss 250 200 u x 150 100 u Udc i 50 0 0 50 100 150 200 250 300 350 400 i,u dc i,u u
More informationChapter 7. The pn Junction
Chapter 7 The pn Junction Chapter 7 PN Junction PN junction can be fabricated by implanting or diffusing donors into a Ptype substrate such that a layer of semiconductor is converted into N type. Converting
More informationSemiconductor Physics and Devices
The pn Junction 1) Charge carriers crossing the junction. 3) Barrier potential Semiconductor Physics and Devices Chapter 8. The pn Junction Diode 2) Formation of positive and negative ions. 4) Formation
More informationIntroduction to Semiconductor Devices
Physics 233 Experiment 48 Introduction to Semiconductor Devices References 1. G.W. Neudeck, The PN Junction Diode, AddisonWesley MA 1989 2. Background notes (Appendix A) 3. Specification sheet for Diode
More informationSemiconductor Junctions
8 Semiconductor Junctions Almost all solar cells contain junctions between different materials of different doping. Since these junctions are crucial to the operation of the solar cell, we will discuss
More informationCarriers Concentration, Current & Hall Effect in Semiconductors. Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India
Carriers Concentration, Current & Hall Effect in Semiconductors 1 Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India http://folk.uio.no/ravi/semi2013 Conductivity Charge
More informationECE 335: Electronic Engineering Lecture 2: Semiconductors
Faculty of Engineering ECE 335: Electronic Engineering Lecture 2: Semiconductors Agenda Intrinsic Semiconductors Extrinsic Semiconductors Ntype Ptype Carrier Transport Drift Diffusion Semiconductors
More informationIntroduction to Semiconductor Devices
Physics 233 Experiment 48 Introduction to Semiconductor Devices References 1. G.W. Neudeck, The PN Junction Diode, AddisonWesley MA 1989 2. Background notes (Appendix A) 3. Specification sheet for Diode
More information6.012 Electronic Devices and Circuits
Page 1 of 1 YOUR NAME Department of Electrical Engineering and Computer Science Massachusetts Institute of Technology 6.12 Electronic Devices and Circuits Exam No. 1 Wednesday, October 7, 29 7:3 to 9:3
More information5. Semiconductors and PN junction
5. Semiconductors and PN junction Thomas Zimmer, University of Bordeaux, France Summary Learning Outcomes... 2 Physical background of semiconductors... 2 The silicon crystal... 2 The energy bands... 3
More informationIsolated atoms Hydrogen Energy Levels. Neuromorphic Engineering I. Solids Energy bands. Metals, semiconductors and insulators Energy bands
Isolated atoms Hydrogen Energy Levels Neuromorphic Engineering I INI404 227103300 Electron in atoms have quantized energy levels Material courtesy of Elisabetta Chicca Bielefeld University, Germany
More informationA semiconductor is an almost insulating material, in which by contamination (doping) positive or negative charge carriers can be introduced.
Semiconductor A semiconductor is an almost insulating material, in which by contamination (doping) positive or negative charge carriers can be introduced. Page 2 Semiconductor materials Page 3 Energy levels
More informationFor the following statements, mark ( ) for true statement and (X) for wrong statement and correct it.
Benha University Faculty of Engineering Shoubra Electrical Engineering Department First Year communications. Answer all the following questions Illustrate your answers with sketches when necessary. The
More informationSemiconductor Physics
Semiconductor Physics Motivation Is it possible that there might be current flowing in a conductor (or a semiconductor) even when there is no potential difference supplied across its ends? Look at the
More informationCLASS 1 & 2 REVISION ON SEMICONDUCTOR PHYSICS. Reference: Electronic Devices by Floyd
CLASS 1 & 2 REVISION ON SEMICONDUCTOR PHYSICS Reference: Electronic Devices by Floyd 1 ELECTRONIC DEVICES Diodes, transistors and integrated circuits (IC) are typical devices in electronic circuits. All
More informationECE 442. Spring, Lecture 2
ECE 442 Power Semiconductor Devices and Integrated circuits Spring, 2006 University of Illinois at Chicago Lecture 2 Semiconductor physics band structures and charge carriers 1. What are the types of
More informationSemiconductors. Semiconductors also can collect and generate photons, so they are important in optoelectronic or photonic applications.
Semiconductors Semiconducting materials have electrical properties that fall between true conductors, (like metals) which are always highly conducting and insulators (like glass or plastic or common ceramics)
More informationUNIVERSITY OF CALIFORNIA, BERKELEY College of Engineering Department of Electrical Engineering and Computer Sciences
UNIVERSITY OF CALIFORNIA, BERKELEY College of Engineering Department of Electrical Engineering and Computer Sciences EE 105: Microelectronic Devices and Circuits Spring 2008 MIDTERM EXAMINATION #1 Time
More informationCEMTool Tutorial. Semiconductor physics
EMTool Tutorial Semiconductor physics Overview This tutorial is part of the EMWARE series. Each tutorial in this series will teach you a specific topic of common applications by explaining theoretical
More informationEE105 Fall 2015 Microelectronic Devices and Circuits: Semiconductor Fabrication and PN Junctions
EE105 Fall 2015 Microelectronic Devices and Circuits: Semiconductor Fabrication and PN Junctions Prof. Ming C. Wu wu@eecs.berkeley.edu 511 Sutardja Dai Hall (SDH) 1 pn Junction ptype semiconductor in
More informationReview of Semiconductor Fundamentals
ECE 541/ME 541 Microelectronic Fabrication Techniques Review of Semiconductor Fundamentals Zheng Yang (ERF 3017, email: yangzhen@uic.edu) Page 1 Semiconductor A semiconductor is an almost insulating material,
More informationDevices. chapter Introduction. 1.2 Silicon Conductivity
chapter 1 Devices 1.1 Introduction The properties and performance of analog bicmos integrated circuits are dependent on the devices used to construct them. This chapter is a review of the operation of
More informationSemiconductor Physics fall 2012 problems
Semiconductor Physics fall 2012 problems 1. An ntype sample of silicon has a uniform density N D = 10 16 atoms cm 3 of arsenic, and a ptype silicon sample has N A = 10 15 atoms cm 3 of boron. For each
More informationCurrent mechanisms Exam January 27, 2012
Current mechanisms Exam January 27, 2012 There are four mechanisms that typically cause currents to flow: thermionic emission, diffusion, drift, and tunneling. Explain briefly which kind of current mechanisms
More informationLECTURE 23. MOS transistor. 1 We need a smart switch, i.e., an electronically controlled switch. Lecture Digital Circuits, Logic
LECTURE 23 Lecture 1620 Digital Circuits, Logic 1 We need a smart switch, i.e., an electronically controlled switch 2 We need a gain element for example, to make comparators. The device of our dreams
More informationDavid J. Starling Penn State Hazleton PHYS 214
Being virtually killed by a virtual laser in a virtual space is just as effective as the real thing, because you are as dead as you think you are. Douglas Adams, Mostly Harmless David J. Starling Penn
More informationSemiconductor Physics. Lecture 3
Semiconductor Physics Lecture 3 Intrinsic carrier density Intrinsic carrier density Law of mass action Valid also if we add an impurity which either donates extra electrons or holes the number of carriers
More informationUNIVERSITY OF CALIFORNIA College of Engineering Department of Electrical Engineering and Computer Sciences. EECS 130 Professor Ali Javey Fall 2006
UNIVERSITY OF CALIFORNIA College of Engineering Department of Electrical Engineering and Computer Sciences EECS 130 Professor Ali Javey Fall 2006 Midterm I Name: Closed book. One sheet of notes is allowed.
More informationA SEMICONDUCTOR DIODE. PN Junction
A SEMICONDUCTOR DIODE PN Junction Analog Electronics Pujianto Department of Physics Edu. State University of Yogyakarta A Semiconductor Devices A Semiconductor devices can be defined as a unit which consists,
More informationMetal Semiconductor Contacts
Metal Semiconductor Contacts The investigation of rectification in metalsemiconductor contacts was first described by Braun [3335], who discovered in 1874 the asymmetric nature of electrical conduction
More informationReview of Semiconductor Physics. Lecture 3 4 Dr. Tayab Din Memon
Review of Semiconductor Physics Lecture 3 4 Dr. Tayab Din Memon 1 Electronic Materials The goal of electronic materials is to generate and control the flow of an electrical current. Electronic materials
More informationPN Junctions. Lecture 7
Lecture 7 PN Junctions Kathy Aidala Applied Physics, G2 Harvard University 10 October, 2002 Wei 1 Active Circuit Elements Why are they desirable? Much greater flexibility in circuit applications. What
More informationIntroduction to Transistors. Semiconductors Diodes Transistors
Introduction to Transistors Semiconductors Diodes Transistors 1 Semiconductors Typical semiconductors, like silicon and germanium, have four valence electrons which form atomic bonds with neighboring atoms
More informationLecture 15  The pn Junction Diode (I) IV Characteristics. November 1, 2005
6.012  Microelectronic Devices and Circuits  Fall 2005 Lecture 151 Lecture 15  The pn Junction Diode (I) IV Characteristics November 1, 2005 Contents: 1. pn junction under bias 2. IV characteristics
More informationObjective: The purpose of these notes is to familiarize students with semiconductors and devices including the PN junction, and the transistors.
 13/4/02C:\lec320.doc H.L.Kwok SEMICONDUCTOR MATERIALS AND DEVICES by H.L. Kwok Objective: The purpose of these notes is to familiarize students with semiconductors and devices including the PN junction,
More informationElectronics The basics of semiconductor physics
Electronics The basics of semiconductor physics Prof. Márta Rencz, Gergely Nagy BME DED September 16, 2013 The basic properties of semiconductors Semiconductors conductance is between that of conductors
More informationSemiconductor Detectors are Ionization Chambers. Detection volume with electric field Energy deposited positive and negative charge pairs
1 V. Semiconductor Detectors V.1. Principles Semiconductor Detectors are Ionization Chambers Detection volume with electric field Energy deposited positive and negative charge pairs Charges move in field
More informationISSUES TO ADDRESS...
Chapter 12: Electrical Properties School of Mechanical Engineering Choi, HaeJin Materials Science  Prof. Choi, HaeJin Chapter 121 ISSUES TO ADDRESS... How are electrical conductance and resistance
More information3.7 Physical Operation of Diodes
10/4/2005 3_7 Physical Operation of Diodes blank.doc 1/2 3.7 Physical Operation of Diodes Reading Assignment: pp. 190200, 203205 A. Semiconductor Materials Q: So, what exactly is a junction diode made
More informationObjective: The purpose of these notes is to familiarize students with semiconductors and devices including the PN junction, and the transistors.
 11/15/02C:\lec320.doc H.L.Kwok SEMICONDUCTOR MATERIALS AND DEVICES by H.L. Kwok Objective: The purpose of these notes is to familiarize students with semiconductors and devices including the PN junction,
More informationSRI VIDYA COLLEGE OF ENGINEERING AND TECHNOLOGY VIRUDHUNAGAR Department of Electronics and Communication Engineering
SRI VIDYA COLLEGE OF ENGINEERING AND TECHNOLOGY VIRUDHUNAGAR Department of Electronics and Communication Engineering Class/Sem:I ECE/II Question Bank for EC6201ELECTRONIC DEVICES 1.What do u meant by
More informationEECS130 Integrated Circuit Devices
EECS130 Integrated Circuit Devices Professor Ali Javey 9/18/2007 P Junctions Lecture 1 Reading: Chapter 5 Announcements For THIS WEEK OLY, Prof. Javey's office hours will be held on Tuesday, Sept 18 3:304:30
More informationLecture 2 Electrons and Holes in Semiconductors
EE 471: Transport Phenomena in Solid State Devices Spring 2018 Lecture 2 Electrons and Holes in Semiconductors Bryan Ackland Department of Electrical and Computer Engineering Stevens Institute of Technology
More informationSection 12: Intro to Devices
Section 12: Intro to Devices Extensive reading materials on reserve, including Robert F. Pierret, Semiconductor Device Fundamentals EE143 Ali Javey Bond Model of Electrons and Holes Si Si Si Si Si Si Si
More informationSpring Semester 2012 Final Exam
Spring Semester 2012 Final Exam Note: Show your work, underline results, and always show units. Official exam time: 2.0 hours; an extension of at least 1.0 hour will be granted to anyone. Materials parameters
More informationSession 6: Solid State Physics. Diode
Session 6: Solid State Physics Diode 1 Outline A B C D E F G H I J 2 Definitions / Assumptions Homojunction: the junction is between two regions of the same material Heterojunction: the junction is between
More informationIntroduction to Electronics and Semiconductor
Introduction to Electronics and Semiconductor 1 Chapter Objectives To study and understand basic electronics. To study and understand semiconductor principles. 2 Definition Electronics is the branch of
More informationSemiconductor Device Physics
1 Semiconductor Device Physics Lecture 3 http://zitompul.wordpress.com 2 0 1 3 Semiconductor Device Physics 2 Three primary types of carrier action occur inside a semiconductor: Drift: charged particle
More informationPHYSICAL ELECTRONICS(ECE3540) CHAPTER 9 METAL SEMICONDUCTOR AND SEMICONDUCTOR HETEROJUNCTIONS
PHYSICAL ELECTRONICS(ECE3540) CHAPTER 9 METAL SEMICONDUCTOR AND SEMICONDUCTOR HETEROJUNCTIONS Tennessee Technological University Monday, November 11, 013 1 Introduction Chapter 4: we considered the semiconductor
More informationSemiconductors (Chất1bán1dẫn)
To describe the properties of ntype and ptype semiconductors and how a pn jun formed To study a diode and the characteristics of diode 11 Atomic Structure Atomic1Structure An atom is the smallest particle
More informationpn JUNCTION THE SHOCKLEY MODEL
The pn Junction: The Shockley Model ( S. O. Kasap, 1990001) 1 pn JUNCTION THE SHOCKLEY MODEL Safa Kasap Department of Electrical Engineering University of Saskatchewan Canada Although the hole and its
More informationCarriers Concentration in Semiconductors  V. Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India
Carriers Concentration in Semiconductors  V 1 Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India http://folk.uio.no/ravi/semi2013 Motion and Recombination of Electrons and
More information